MECHANICAL PROPERTIES AND DURABILITY OF ABSTRACT This paper presents a study on the mechanical...
Embed Size (px)
Transcript of MECHANICAL PROPERTIES AND DURABILITY OF ABSTRACT This paper presents a study on the mechanical...
MECHANICAL PROPERTIES AND DURABILITY OF CONCRETE MADE WITH HIGH-VOLUME FLY ASH BLENDED CEMENTS USING A COARSE FLY ASH
N. Bouzouba1*, M. H. Zhang1, and V. M. Malhotra1
International Centre for Sustainable Development of Cement and Concrete (ICON) CANMET/Natural resources Canada
405 Rochester Street, Ottawa, ON, Canada K1A 0G1
Cement and Concrete Research, Vol. 31, No. 3, Oct. 2001, pp. 1393-1402. Keywords: Blended cement, Compressive strength, Concrete, Durability, Fly ash.
ABSTRACT This paper presents a study on the mechanical properties and durability of concrete made with a high-volume fly ash blended cement using a coarse fly ash that does not meet the fineness requirement of ASTM C 618. The results were compared with those of the HVFA concrete in which unground fly ash had been added at the concrete mixer. The properties of the fresh concrete determined included the slump, air content, slump loss, stability of air content, bleeding, and setting time; those of the hardened concrete investigated included the compressive strength, flexural- and splitting-tensile strengths, Youngs modulus of elasticity, drying shrinkage, resistance to abrasion, chloride-ion penetration, freezing and thawing cycling, and to de-icing salt scaling. The results show that except for the resistance of the concrete to the de-icing salt scaling, the mechanical properties and the durability of concrete made with this blended cement were superior to the concrete in which the unground fly ash and the cement had been added separately at the mixer. The production of HVFA blended cements, therefore, offers an effective way for the utilization of coarse fly ashes that do not otherwise meet the fineness requirements of ASTM C 618.
In the mid 1990s, CANMET undertook a major research project to develop blended cements
incorporating high volumes of ASTM Class F fly ash. The objectives of the project were to
reduce CO2 emissions from the production of cement clinker, to reduce the consumption of raw
materials such as limestone and clay, and to contribute to a cleaner environment through the
recycling of waste materials such as fly ash. The blended cement developed is made by
intergrinding approximately 55% (weight percentage) of ASTM Class F fly ash and 45% of
ASTM Type I or Type III cement clinker together with a small amount of gypsum, and in some
cases with a small amount of dry superplasticizer [1-6].
The results from previous investigations  had shown that, in general, the compressive strength
and resistance to chloride-ion penetration of the concrete made with high-volume fly ash
(HVFA) blended cements were superior or equal to that of the concrete in which the cement and
the unground fly ash had been added as separately batched materials at a concrete mixer. For
high-volume fly ash blended cements made with fine fly ashes, the improvement in the
mechanical properties and durability characteristics was marginal, while for the HVFA blended
cements made using a coarse fly ash, the improvement was significant.
This paper presents a study on the mechanical properties and durability of concrete made with a
high-volume fly ash blended cement using a coarse fly ash that does not meet the fineness
requirements of ASTM C 618. The results are compared with those of the HVFA concrete
where unground fly ash had been added at the concrete mixer, and control portland cement
concrete. The control mixtures were made with a commercially available ASTM Type III
cement and, a normal-portland cement (LPC) produced in the laboratory that meet the
requirements of ASTM Type III cement. The properties of the fresh concrete determined
included the slump, air content, slump loss, stability of air content, bleeding, and setting time;
those of the hardened concrete investigated included the compressive strength, flexural- and
splitting-tensile strengths, Youngs modulus of elasticity, drying shrinkage, resistance to
abrasion, chloride-ion penetration, freezing and thawing cycling, and to de-icing salt scaling.
2.1. Portland Cement Clinker
Portland cement clinker was obtained from a cement plant in Montreal area, and this clinker is
used by the cement company to produce ASTM Type III cement. Its specific gravity and
chemical composition are given in Table 1.
2.2. Portland Cement
A commercially available ASTM Type III portland cement from the same company that
provided the clinker was used for the control concrete. Its chemical composition and physical
properties are given in Table 2.
2.3. Fly Ash
A fly ash from Genesee, Alberta was used in this study. Its physical properties and chemical
composition are given in Table 1. The fly ash has a relatively low Blaine fineness of 2120
cm2/g, and the amount of the ash retained when wet sieved on a 45 :m sieve was 36.5%. This
ash, therefore, fails to meet the fineness requirement of ASTM C 6181. The ash has a relatively
low specific gravity, and this is primarily related to a large numbers of plerospheres that are
hollow particles filled with smaller spheres in the sample. The ash has a CaO content of 5.8%
and an alkali content (Na2O equivalent) of 3.6%. This ash meets the chemical requirements of
ASTM Class F fly ash.
1ASTM C 618 requires that the amount retained when wet-sieved on a 45:m sieve be less than 34%.
A sulphonated, naphthalene-formaldehyde condensate type of superplasticizer in a powder form
was used in all the concrete mixtures.
2.5. Air-Entraining Admixture
A synthetic resin type air-entraining admixture (AEA) was used in all the mixtures.
A crushed granite with a maximum nominal size of 19 mm was used as the coarse aggregate, and
a local natural sand was used as the fine aggregate. Both the coarse and fine aggregates were
separated into different size fractions and recombined to a specific grading shown in Table 3.
The coarse and fine aggregates each had a specific gravity of 2.70, and water absorptions of 0.5
and 0.8%, respectively.
3. Production of the Cements
The production of the HVFA blended cement that meets the requirements of ASTM C 1157 GU
involved two stages; these consisted of producing a portland cement with a Blaine fineness of
4000 cm2/g (LPC), and then intergrinding 45% (by mass) of the above cement with 55% of the
fly ash for 80 minutes. The cement LPC was produced by grinding 97% clinker together with
3% gypsum. Before the clinker was fed to the grinding mill, it was crushed and sieved so that all
the particles were less than 0.6 mm in size. The two cements produced are designated as
Blended cement produced using Genesee fly ash = BCG
Laboratory-produced, normal-portland cement = LPC
A ceramic grinding mill, 420 mm in length and 500 mm in diameter with a grinding capacity of
approximately 10 kg material, was used for the production of the cements. A combination of 35
kg of large ceramic cylinders (30-mm thick and 30-mm diameter) and 35 kg of medium ceramic
cylinders (20-mm thick and 20-mm diameter) was used for grinding. The weight ratio of the
materials to be ground to the grinding media was 1:7.
4. Mixture Proportions
Two high-volume fly ash concrete and two control portland-cement concrete mixtures were
made. For the HVFA concrete, one concrete mixture was made in which unground fly ash was
added at the concrete mixer, and the other mixture was made with the blended cement. The
proportions of the concrete mixtures are summarized in Table 4.
For all the mixtures, the coarse and fine aggregates were weighed in a room dry condition. The
coarse aggregate was then immersed in water for 24 hours. The excess water was decanted, and
the water retained by the aggregates was determined by the weight difference. A predetermined
amount of water was added to the fine aggregate that was then allowed to stand for 24 hours.
A water-to-cementitious materials ratio of 0.32 was used for the fly ash concrete mixtures. The
water-to-cement ratios of the control concrete made with the commercially available ASTM
Type III cement and the LPC cement were 0.42 and 0.40, respectively; these water-to-cement
ratios were chosen to obtain concrete with a 28-day compressive strength similar to that of
concrete made with the HVFA blended cement.
5. Preparation and Casting of Test Specimens
All the concrete mixtures were mixed for five minutes in a laboratory counter-current mixer, and
for each concrete mixture two batches were made.
5.1. Batch A
Twenty-four 102x203-mm and six 152x305-mm cylinders were cast for each concrete mixture.
The 102x203-mm cylinders were used for the determination of the compressive strength and the
resistance to the chloride ion-penetration of the concrete, and the 152x305-mm cylinders were
used for determining the splitting-tensile strength and the Young's modulus of elasticity. One
container of approximately 7 L capacity was filled with the fresh concrete for determining the
bleeding, and one 152x152x152-mm mould was filled with mortar obtained by sieving the fresh
concrete for determining the setting times of concr